|Experimental Chemistry|| Main project page|
Previous entry Next entry
Preparing PVOH film (using 0.5 g of 22,000 MW PVOH and 5 ml of water at around 70 deg Celsius)PVOH Cross-linking with 0.25 ml of glutaraldehyde, 100 % exchange Na-MT, 50 % exchange Na-MT, and γ Fe3O4 coated Na-MT (in a ratio of 1.5:1 to make a magnet absorbent) in 2 g Na-MT would be prepared.
PVOH + Glutaraldehyde: 0.5 g of PVOH (MW of 22,000) in 5 ml of water solution was prepared, by heating the solution at 80 degrees Celsius and was stirred until completely dissolved. Then, 0.25 ml of glutaraldehyde was added (by using the P-1000) once the solution was cooled at room temperature, under constant stirring. The resultant solution was allowed to stay in the fume hood for up to 48 hrs for the film production to occur.
100 % Exchange Sodium Montmorillonite, NaMT: Mass of the surfactant, DMHdIBr, used was 0.7390 g, was added into 25 ml of water (HPLC grade), in addition to 2.004 g clay (NaMT) and 25 ml ethanol, under constant stirring for a week (7-days).
50 % Exchange Sodium Montmorillonite, NaMT: Mass of the surfactant, DMHdIBr, used was 0.3690 g, was added to 25 ml of hplc graded water, in addition to 2.000 g of clay (NaMT), and 25 ml ethanol, under constant stirring for a week (7-days).
γFe3O4 Coated NaMT (magnet absorbent) 1.5:1 ratio : To prepare this solution, 1.04 g of Iron(II) chloride was mixed with 0.5 g of Iron(II) sulfate in 40 ml of water solution. 2 g of the clay, NaMT was also used in presence of 2.67 g, NaOH in 10 ml solution, that was aided drop wise.
100 % Exchange Sodium Montmorillonite, NaMT: Theoretical Calculations for DMHDIBr- Surfactant used: (0.92 meq v/g)* (2g clay) * (1eqv/ 1000meqv) * (1 mol surfactant/ 1eqv ) * (401.47 g/ 1 mol of surfactant) =0.7387 g of surfactant
50 % Exchange Sodium Montmorillonite, NaMT: Theoretical Calculations for DMHDIBr- Surfactant used:
1/2 * (0.7387 g) = 0.3695 g of surfactant used.
For glutaraldehyde Crosslinking, mass of PVOH = 0.4995 g, Vol of Glutaraldehyde, 0.4 weight % solution = 0.25 ml
For 100 % Exchange: mass of surfactant used = 0.7390 g, vol. of water (hplc grade) = 25 ml, vol. of ethanol = 25 ml, mass of clay (Na-MT) = 2.004 g
For 50% Exchange: mass of surfactant used = 0.3690 g, vol. of water (hplc grade) = 25 ml, vol. of ethanol = 25 ml, mass of clay (Na-MT) = 2.000 g
FeCl2 = 1.04 g, FeSO4 = 0.5 g, mass of Na-MT = 2 g, NaOH = 2.67 g in 10 ml of water added drop wise. mass of filter paper = 0.33684 g
Follow the NASA article on glutaraldehyde cross-linking
Clay-iron oxide, magnetic composite exhibited magnetic properties.